Reinforcing effect of poly(furfuryl alcohol) in cellulose-based porous materials
- 615 Downloads
The mechanical reinforcement of porous materials made of microfibrillated cellulose by in situ polymerisation of furfuryl alcohol prior to freeze-drying from aqueous slurry was studied. Besides a slight improvement in the modulus of elasticity measured in compression testing, no beneficial effects of furfuryl alcohol addition on porous materials produced from microfibrillated cellulose derived from bleached softwood pulp were observed. By contrast, when microfibrillated cellulose containing substantial amounts of residual non-cellulosic cell wall polymers, termed microfibrillated lignocellulose, was used, clear mechanical reinforcement effects due to furfuryl alcohol addition were measured. By means of SEM, significantly improved wetting of the cellulosic fibrillary architecture of porous materials with furfuryl alcohol was observed for microfibrillated lignocellulose compared to microfibrillated cellulose. It is proposed that the specific surface-chemical character of microfibrillated lignocellulose enables wetting of fibrils with furfuryl alcohol, thus providing micron fibre-reinforced structures with improved strength after in situ polymerisation. Besides mechanical properties, the density and thermal stability of cellulose-based porous materials were found to increase with increasing amounts of furfuryl alcohol added to the initial reaction slurry.
KeywordsCompressive strength Freeze-drying Furfuryl alcohol Microfibrillated cellulose Porous material
Low-density cellulosic materials are of interest due to their high inner surface, high toughness, and thermally insulating properties (Aulin et al. 2010; De France et al. 2017; Lavoine and Bergstrom 2017; Srinivasa et al. 2015; Wicklein et al. 2015). At laboratory scale, a bottom-up approach based on cellulose solutions or suspensions of microfibrillated cellulose dried in supercritical carbon dioxide or by means of freeze-drying is most commonly followed. Recently, a top-down approach involving the removal of lignin from solid wood and subsequent freeze-drying has been proposed (Li et al. 2018). Using this approach, anisotropic features similar to special ice-templating (Lee and Deng 2011) and densification methods (Plappert et al. 2017) are obtained. Potential applications of low-density cellulosic solids comprise examples as diverse as thermal insulation (Li et al. 2018; Plappert et al. 2017; Wicklein et al. 2015), packaging (Svagan et al. 2011; 2010; 2008), oil adsorption (Korhonen et al. 2011; Tarrés et al. 2016; Zhang et al. 2014), or supercapacitors (Li et al. 2016; Zu et al. 2016).
As shown by Sehaqui et al. (2010), (2011), the density of isotropic porous microfibrillated cellulose-based solids is the main determinant of mechanical strength and stiffness. Beyond that, combinations of microfibrillated cellulose and polymeric binders or matrices may provide further improvements in mechanical stability. Due to the inherent hydrophilicity of native cellulose and due to the fact that microfibrillated cellulose is typically produced by means of fibrillation in aqueous state, water soluble systems are of primary interest. In previous studies (Ago et al. 2016; Svagan et al. 2011; 2008), starch has been successfully used to produce fully biodegradable high performance microfibrillated cellulose foams. Furthermore, water soluble synthetic polyvinyl alcohol (PVOH) has been used to prepare PVOH-cellulose hybrid aerogels (Zheng et al. 2014). When using polymers insoluble in water, solvent exchange with organic solvents is applied (Pircher et al. 2014). Finally, chemical cross linking (Kim et al. 2015; Yang and Cranston 2014) may also provide additional stabilisation.
With regard to chemical cross-linking, furfuryl alcohol (FA) has been repeatedly used in bio-based foams on the basis of either lignin (Tondi et al. 2016) or tannins (Reyer et al. 2016; Szczurek et al. 2016). Modification of solid wood with FA, often referred to as “furfurylation”, has been known since decades. In recent years, new furfurylation processes applying new catalytic systems and process additives have been developed. As reported by Lande et al. (2008), the properties of furfurylated wood strongly depend on the retention of polymerised furfuryl alcohol (PFA) in the wood structure. At high modification levels, i.e. high retention of PFA, a whole bunch of properties are improved. This particularly involves hardness, resistance to microbial decay and insect attack, dimensional stability as well as bending strength and modulus of elasticity. FA may be considered a green chemical, since it is industrially produced by hydrogenation of furfural, which is itself typically derived from waste bio-mass such as corncobs or sugar cane bagasse (Mariscal et al. 2016). Despite its bio-based character, FA is attractive due to its high reactivity and the option of processing in mixtures with aqueous systems (Gandini et al. 2016). Even though the process of wood furfurylation has been known for a long time, the exact mechanisms of how FA interacts with wood constituents during in situ polymerization are not yet fully understood. Usually, furfurylation is carried out by impregnating wood with a mixture of FA and catalysts after which the impregnated wood is heated to induce polymerisation. As shown by Nordstierna et al. (2008), aromatic lignin units with hydroxyl groups are highly reactive towards the polymerising PFA chain and the polymerising FA was found to covalently bind to lignin model compounds. Thus, this supports the hypothesis that the furan polymer in furfurylated wood is similarly grafted to wood lignin. Ehmcke et al. (2017) used cellular ultraviolet microspectrophotometry (UMSP) to analyze chemical alterations of individual cell wall layers of furfurylated radiata pine. The UV-absorbance of modified samples increased significantly compared to the untreated controls, indicating a strong polymerization of the aromatic compounds. Highest UV-absorbances were found in areas with the highest lignin concentration. The UMSP images of individual cell wall layers again suggest the occurrence of condensation reactions between lignin and FA. However, the extent of covalent linkages between PFA and lignin remains largely unknown. Apart from furfurylation of solid wood, several studies reporting on composite materials from cellulose-based fibres and PFA can be found in literature. Pranger and Tannenbaum (2008) as well as Pranger et al. (2012) prepared nanocomposites by in situ polymerisation of furfuryl alcohol in the presence of low amounts of cellulose nanowhiskers (CNW). Sulfonic acid residues present at the CNW surface were found to catalyse FA polymerisation. Prepared CNW/PFA nanocomposites exhibited increased thermal stability as well as enhanced breaking strength and toughness as compared to unfilled and filled PFA systems previously described in literature. Another group of authors used cellulose extracted from cotton (Motaung et al. 2016) and flax fibres (Motaung et al. 2018) for the preparation of cellulose/PFA composites. Again, higher thermal stability and better flexural strength and modulus were found for cellulose/PFA composites as compared to the neat PFA matrix.
In the present study, the option of improving the mechanics of porous cellulosic materials by means of in situ polymerisation of FA is evaluated. Two variants of microfibrillated cellulose with known differences in surface chemistry due to differing chemical composition were used in order to ensure optimum compatibility between the cellulosic scaffold and the in situ polymerised FA-based binder.
Materials and methods
Preparation of porous materials
For the preparation of porous materials, two types of microfibrillated cellulose were used, which are both described in more detail elsewhere (Winter et al. 2017). Briefly, microfibrillated cellulose produced by mechanical refining of bleached softwood kraft pulp, termed MFC, was purchased from the University of Maine. According to the manufacturer, the pulp used as a starting material for MFC preparation comprises of 80–85 wt% cellulose, 15–20 wt% hemicelluloses and < 0.1 wt% residual lignin (kappa number ~ 0.5). Fibrils have a nominal width of 50 nm and a length of up to several hundred microns. In parallel, organosolv-pulped beech wood-derived microfibrillated cellulose with 8.5% residual lignin content and a hemicellulose content of around 10 wt%, termed MFLC (microfibrillated lignocellulose), was used. With a crystallinity index of 0.70 for MFC and 0.74 for MFLC, both cellulose materials used show similar crystallinity (Winter et al. 2017). The choice of these two fibril variants was motivated by their repeatedly observed differences in surface-chemical properties, with MFLC being essentially less polar than MFC (Ballner et al. 2016; Herzele et al. 2016; Winter et al. 2017; Yan et al. 2016). Aqueous fibril slurries were adjusted to a solid content of 4 wt%. Furfuryl alcohol (FA, 98% purity, Aldrich) and appropriate aliquots of maleic anhydride (≥ 98% purity, Fluka), i.e. 5 wt% with regard to the amount of FA used, were added to the slurry. The mass fraction of FA (related to the overall solids of the mixture) was set to 0.00, 0.03, 0.06, 0.11, 0.20, 0.33 and 0.50. Additionally, a sample of pure PFA was prepared for IR spectroscopy and TGA experiments. After mixing with a hand blender (T 10 basic Ultra Turrax, IKA-Werke, Staufen, Germany) operated at 20.500 min−1, the mixtures were transferred to 2 ml Eppendorf tubes and placed in a drying oven at 80 °C for 24 h. Thereafter, the tubes were opened and all mixtures were frozen in a cold box (B 35-85, Fryka-Kältetechnik, Esslingen, Germany) at − 80 °C. Finally, the frozen samples were transferred to a freeze-dryer (Alpha 1-2 LDplus, Martin Christ Gefriertrocknungsanlagen, Osterode am Harz, Germany) and lyophilized at 0.37 mbar (corresponding to a temperature of − 30 °C) for 72 h.
Scanning electron microscopy (SEM) was carried out with gold-coated specimens in a Quanta™ 250 FEG from FEI in high-vacuum secondary electron mode.
ATR-Fourier-transform infrared spectra were obtained with a Perkin–Elmer Frontier FT-IR spectrometer equipped with an attenuated total reflection (ATR) Zn/Se crystal. For FT-IR measurements, one specimen was cut from each of the lyophilized samples and scanned twice from 4000 to 650 cm−1 at 4 cm−1 resolution to calculate an average spectrum. All spectra were normalized for comparison and smoothed by applying a Savitzky–Golay filter (third degree polynomial at an interval of 25).
Thermogravimetric analysis (TGA) was carried out using a Netzsch TGA device (TG 209 F1 Iris, Netzsch, Selb, Germany). TGA specimens weighing between 2 and 3 mg were prepared from the freeze-dried material and placed into an 85 µl aluminium oxide crucible. TGA runs were conducted from room temperature to 800 °C with a heating rate of 10 K min−1 and a nitrogen flow rate of 20 ml min−1. Two samples were measured for each specimen group.
Compression testing was done on a Zwick-Roell Z020 universal testing machine equipped with a 500 N load cell. Tests were carried out with cylindrical specimens (diameter = 8 mm, height = 6 mm) at a deformation rate of 1 mm min−1. The apparent modulus of elasticity was determined by fitting a linear regression to the first, quasi-linear portion of the stress–strain curve. As suggested by Christensen (2008), yield stress was determined from the second derivative of the stress strain curve. It was assumed that the strain at which the second derivative, d2σ/dε2, achieves a maximum value (εy) is a transition point and the associated stress (σy) was taken as the yield stress. This point designates the transition from the previous nearly ideally elastic behaviour to the following behaviour approaching perfectly plastic flow. In cases where a clear stress maximum was present, this local stress maximum was taken as the yield stress for practical reasons.
Results and discussion
Microstructure and density of porous materials
IR-spectroscopy and thermogravimetric analysis
Pure MFC specimens show a modulus of elasticity of 2435 ± 750 kPa and a yield stress of 98 ± 29 kPa. By comparison, pure MFLC shows lower performance with 2005 ± 712 kPa for the modulus and 83 ± 25 kPa for yield stress, respectively, in spite of slightly higher density values for the latter material (Fig. 5). Addition of FA has different effects on the two variants of fibrillated material used. For MFC, addition of FA results in an increase in variability of the modulus of elasticity, and a trend towards higher values. However, no systematic correlation is apparent, or, if present, obscured by high variability. As for yield stress, no significant effect of the presence of PFA in the specimens is observed. By contrast, very clear effects were observed when MFLC instead of MFC was used. Again, a very significant increase in the variability of the modulus of elasticity is observed upon addition of FA. Even so, a positive effect of FA addition on the modulus is obvious. In the variant with highest content of PFA (50% MFLC, 50% PFA), the average modulus of elasticity is 6828 ± 1783 kPa, which corresponds to a roughly threefold increase compared to unreinforced MFLC. With regard to compressive yield stress, effects of FA addition are also evident. In spite of high variability, an initial linear increase of yield stress with increasing amounts of FA added is discernible, reaching maximum values of 177 ± 26 kPa at 33% content of PFA. For the variant with highest PFA content, a decrease in yield stress is observed. To summarise the results shown in Fig. 10 it can be said that the addition of FA has clearly positive effects on the compressive performance of freeze-dried MFLC, whereas this is hardly the case for MFC.
It is thus proposed that the cellular architecture of freeze-dried MFLC foams is significantly altered by FA addition. SEM images of freeze-dried specimens with FA addition (Fig. 3) confirm this assumption and also indicate a potential mechanism behind the significantly different behaviour of MFC and MFLC observed in this regard.
The results shown in the present study clearly demonstrate that a simple approach of reinforcing porous MFC architectures with PFA by means of in situ polymerisation in aqueous slurry and subsequent freeze-drying is not feasible with standard MFC produced from bleached wood pulp, as there is insufficient wetting between the two phases (cellulose and furfuryl alcohol) of the compound. By contrast, MFLC containing substantial amounts of residual non-cellulosic wood polymers, affords good wettability with furfuryl alcohol and, consequently, a more homogeneous distribution of polymerized FA throughout the lignocellulose scaffold. Although not analysed more closely, the results of the present study thus indicate a strong affinity of FA towards non-cellulosic cell wall constituents during in situ polymerization, ultimately resulting in excellent mechanical reinforcement of porous structures after freeze-drying. Thus modification of MFLC with furfuryl alcohol and subsequent freeze-drying provides a way to prepare lightweight lignocellulosic materials with improved strength and stiffness. In future, such porous materials could provide a bio-based alternative to polystyrene-based foams which are currently extensively used in thermal insulation and packaging applications.
Open access funding provided by University of Natural Resources and Life Sciences Vienna (BOKU).
- Gindl W, Müller U, Teischinger A (2003) Transverse compression strength and fracture of spruce wood modified by melamine-formaldehyde impregnation of cell walls. Wood Fiber Sci 35:239–246Google Scholar
- Guigo N, Mija A, Zavaglia R, Vincent L, Sbirrazzuoli N (2009) New insights on the thermal degradation pathways of neat poly(furfuryl alcohol) and poly(furfuryl alcohol)/SiO < inf > 2</inf > hybrid materials. Polym Degrad Stab 94:908–913. https://doi.org/10.1016/j.polymdegradstab.2009.03.008 CrossRefGoogle Scholar
- Plappert SF, Nedelec J-M, Rennhofer H, Lichtenegger HC, Liebner FW (2017) Strain hardening and pore size harmonization by uniaxial densification: a facile approach toward superinsulating aerogels from nematic nanofibrillated 2,3-dicarboxyl cellulose. Chem Mater 29:6630–6641. https://doi.org/10.1021/acs.chemmater.7b00787 CrossRefGoogle Scholar
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.